MIXED-MODE CRACK PROPAGATION
IN FUNCTIONALLY GRADED MATERIALS
Jeong-Ho Kim1 and Glaucio H. Paulino2
Department of Civil and Environmental Engineering, University of Connecticut, Storrs, CT 06269, USA
Department of Civil and Environmental Engineering University of Illinois, Urbana, IL 61801, USA
Increasing performance demand in a variety of applications of functionally graded materials makes the
fracture behavior of such materials very important for assessing and enhancing the structural integrity. This
paper briefly reviews previous works on FGMs and mainly focuses on mixed-mode crack growth in FGMs.
In this paper, automatic simulation of crack propagation in functionally graded materials is performed by
means of a remeshing algorithm in conjunction with the finite element method. The crack propagation is
performed under mixed-mode loading. Each step of crack growth simulation consists of the calculation of the
mixed-mode stress intensity factors by means of a novel formulation, so-called non-equilibrium formulation,
of the interaction integral method, determination of the crack growth direction based on a specific fracture
criterion, and local automatic remeshing along the crack path. A specific fracture criterion is tailored for
FGMs based on the assumption of local homogenization of asymptotic crack-tip fields in FGMs. The present
approach uses a user-defined crack increment at the beginning of the simulation. Crack trajectories obtained
by the present numerical simulation are compared with available experimental results. The present work
provides a basis for further investigation on cracked FGMs under thermo-mechanical loadings.
FGMs are multifunctional composites involving spatially varying volume fractions of constituent
materials, thus providing a graded microstructure, macroproperties [1,2,3]. These materials were
introduced to take advantage of ideal behavior of its material constituents. For instance, partially
stabilized zirconia (PSZ) shows a high resistance to heat and corrosion, and CrNi alloy has high
mechanical strength and toughness as illustrated in Figure 1 . FGMs have been applied to the
following applications: thermal barrier coatings ; first-wall composites in nuclear fusion and
fast breeder reactors ; piezoelectric and thermoelectric devices ; graded refractive index
materials ; thermionic converters ; dental and other implants [10,11]; fire retardant doors
; graded cathodes in solid oxide fuel cells (SOFCs) ; and other applications [2,3].
Figure 1 Micrograph illustrating graded transition region between CrNi alloy and partially
stabilized zirconia (PSZ) .
Due to multifunctional capabilities, FGMs have been investigated for various damage and failure
mechanisms under mechanical or thermal loads, and static, dynamic or fatigue loads, etc [2,3].
2 SIMULATION OF CRACK PROPAGATION
Automatic crack propagation in FGMs is performed by means of the I-FRANC2D (Illinois-
FRANC2D) code . The present code is based on FRANC2D (FRacture Analysis Code 2D)
, which was originally developed at Cornell University. The extended capabilities of I-
FRANC2D consist of special graded elements to model nonhomogeneous materials, and fracture
parameters for FGMs (such as SIFs) which are used to determine crack initiation and to predict
crack initiation angles. Finite element simulation of automatic crack propagation involves
successive steps. Figure 2 illustrates automatic crack propagation procedure at each step.
FEA SIFs θ0 & ∆a
Automatic crack propagation cycle
Local update Delete elements
Continue remeshing crack geometry along crack path
Figure 2 Automatic crack propagation procedure used in the I-FRANC2D code.
3 THE INTERACTION INTEGRAL METHOD
The interaction integral (M-integral) method is an accurate scheme to evaluate SIFs in FGMs
[16,17]. We adopt a non-equilibrium formulation [14,18], which uses displacement and strain
fields developed for homogeneous materials, and employ the non-equilibrium stress fields
σ aux = C ( x ) ε aux , where C ( x ) is the FGM stiffness tensor, σ aux is the auxiliary stress, and ε aux
is the auxiliary strain. The interaction integral is derived from the path-independent J-integral 
for two admissible states of a cracked elastic FGM body. The M-integral, based on the non-
equilibrium formulation, is obtained as [14,18]
M = (σ ij uiaux + σ ij ui ,1 − σ ik ε ik δ1 j )q, j dA + (σ ij , j ui ,1 − Cijkl ,1ε klε ij )q dA ,
aux aux aux aux
where the underlined term is a non-equilibrium term, which appears due to non-equilibrium of the
auxiliary stress fields, and must be considered to obtain converged solutions.
The relationship between M-integral and SIFs (KI,KII) is given by
M = 2( K I K Iaux + K II K II ) / Etip ,
where Etip = Etip for plane stress and Etip = Etip /(1−ν 2 ) for plane strain. The mode I and mode II SIFs
are decoupled and are evaluated as follows:
K I = M (1) Etip / 2, ( K Iaux = 1.0, K II = 0.0)
K II = M (2) Etip / 2, ( K Iaux = 0.0, K II = 1.0)
The relationships of eqn (3) are the same as those for homogeneous materials  except that, for
FGMs, the material properties are evaluated at the crack-tip location .
4 A FRACTURE CRITERION
The singularity (r-1/2) and angular functions of asymptotic stress fields for FGMs are the same as
for homogeneous materials . This local homogenization allows the use of fracture criteria
originally developed for homogeneous materials. Here we adopt the maximum energy release
rates criterion proposed by Hussain et al. . The energy release rate is given by 
2 θ /π
4 1 1− π /θ
G(θ ) = * (1 + 3cos2 θ )KI2 + 8sinθ cosθ KI KII + (9 − 5cos2 θ )KII .
1+ π /θ
Etip 3 + cos2 θ
Then the crack initiation angle θ 0 is obtained from 
∂G (θ ) / ∂θ = 0, ∂ 2G (θ ) / ∂θ 2 < 0 ⇒ θ = θ 0 . (5)
The crack initiation condition is given by
G (θ 0 ) = Gc ( x ) , (6)
where Gc ( x ) is the critical energy release rate function given by
Gc = K Ic ( x ) / Etip .
2 * (7)
5 EXAMPLE: CRACK GROWTH IN AN EPOXY/GLASS FGM BEAM
Rousseau and Tippur  investigated crack growth behavior of a crack normal to the material
gradient in an epoxy/glass (50 vol%) FGM beam subjected to four-point bending. Figure 4 shows
specimen geometry and boundary conditions (BCs) of the FGM beam with a crack located at
ξ=0.37. Table 1 shows the numerical values of material properties at interior points in the graded
region. Material properties in the intermediate regions vary linearly.
Epoxy 37 Glass-rich
0 ξ 1 t=6
5 L=120 5
Figure 4: Geometry and BCs of the epoxy/glass FGM beam
Table 1: Material properties (Young's modulus (E), Poisson's ratio (ν) and fracture toughness
(KIc)) at interior points in the graded region.
ξ E(MPa) ν KIc (MPam1/2)
0.00 3000 0.35 1.2
0.17 3300 0.34 2.1
0.33 5300 0.33 2.7
0.58 7300 0.31 2.7
0.83 8300 0.30 2.6
1.00 8600 0.29 2.6
The following data are used for the FEM analyses: plane stress, a/W=0.25, t=6 mm,
P=Pcr(a+n∆a, X), where n refers to the number of crack propagation increments, ∆a denotes a
crack increment, and X=(X1,X2) denotes crack locations. Figure 5(a) compares experimental results
for crack trajectory with those of numerical simulation (∆a=1mm). There is good agreement
between two results. Moreover, experimental and numerical results for the crack initiation angle at
the initial step are in good agreement, i.e. θexp=7 and θnum=6.98 , respectively. Figures 5(b) and
5(c) show finite element discretizations at the initial and final steps, respectively, of crack
propagation considering ∆a=1mm.
(a) (b) (c)
Figure 5 Experimental and numerical results: (a) Comparison of crack trajectory in the region
0 ≤ W ≤ 16.5mm ; finite element discretizations at the (b) initial (step 0) and (c) final step (step
16) of crack propagation .
This paper investigates fracture behavior of FGMs under mechanical loading by performing
automatic simulation of crack propagation by means of a remeshing scheme in conjunction with
the finite element method. Based on local homogenization, we use the maximum energy release
rate criterion. Crack trajectories obtained by this fracture criterion agree well with available
experimental results for homogeneous and FGMs. The computational scheme developed here
serves as a guideline for fracture experiments on FGM specimens (e.g. initiation toughness and R-
We gratefully acknowledge the support from the NASA Ames Research Center, NAG 2-1424
(Chief Engineer, Dr. Tina Panontin), and the National Science Foundation (NSF) under grant
CMS-0115954 (Mechanics and Materials Program).
 Hirai T. Functionally gradient materials and nanocomposites. In Holt JB, Koizumi M, Hirai T,
and Munir ZA, editors, Proceedings of the Second International Symposium on Functionally
Gradient Materials, volume 34 of Ceramic Transactions, pages 11-20, Westerville, Ohio,
1993. The American Ceramic Society.
 Suresh S and Mortensen AQ. Fundamentals of Functionally Graded Materials. IOM
Communications Ltd, London, 1998.
 Paulino GH, Jin ZH, and Dodds RH Jr. Failure of functionally graded materials. In
Karihaloo B and Knauss WG, editors, Comprehensive Structural Integrity, volume 2, Chapter
13. Elsevier Science, 2003.
 Ilschner B. Processing-microstructure-property relationships in graded materials. Journal of
the Mechanics and Physics of Solids, 44(5):647--656.
 Hirano T, Teraki J, and Yamada T. On the design of functionally gradient materials. In
Yamanouochi M, Koizumi M, Hirai T, and Shiota I, editors, Proceedings of the First
International Symposium on Functionally Gradient Materials, pages 5-10, Sendai, Japan,
 Igari T, Notomi A, Tsunoda H, Hida K, Kotoh T, and Kunishima S. Material properties of
functionally gradient material for fast breeder reactor. In Yamanouochi M, Koizumi M, Hirai
T, and Shiota I, editors, Proceedings of the First International Symposium on Functionally
Gradient Materials, pages 209-214, Sendai, Japan, 1990.
 Tani J and Liu GR. Surface waves in functionally gradient piezoelectric plates. JSME
International Journal Series A (Mechanics and Material Engineering), 36:152-155, 1993.
 Koike Y. Graded-index and single mode polymer optical fibers. In Chiang LY, Garito AG, and
Sandman DJ, editors, Electrical, Optical, and Magnetic Properties of Organic Solid State
Materials, volume 247, page 817, Materials Research Society Proceedings, Pittsburgh, PA,
 Desplat JL. Recent development on oxigenated thermionic energy converter - Overview. In
Proceedings of the Fourth International Symposium on Functionally Gradient Materials,
Tsukuba City, Japan, 1996.
 Watari F, Yokoyama A, Saso F, Uo M, Ohkawa S, and Kawasaki T. EPMA elemental
mapping of functionally graded dental implant in biocompatibility test. In Proceedings of the
Fourth International Symposium on Functionally Gradient Materials, Tsukuba City, Japan,
 Oonishi H, Noda T, Ito S, Kohda A, Yamamoto H, and Tsuji E. Effect of hydroxyapatite
coating on bone growth into porous titanium alloy implants under loaded conditions. Journal
of Applied Biomaterials, 5(1):23-27, 1994.
 Getto H and Ishihara SJ. Development of the fire retardant door with functional gradient
wood. In Proceedings of the Fourth International Symposium on Functionally Gradient
Materials, Tsukuba City, Japan, 1996.
 Hart NT, Brandon NP, Day MJ, and Shemilt JE. Functionally graded cathodes for solid oxide
fuel cells. Journal of Materials Science, 36:1077-1085, 2001.
 Kim JH. Mixed-mode crack propagation in functionally graded materials. Ph.D. Thesis,
University of Illinois at Urbana-Champaign, Illinois, 2003.
 Wawrzynek PA. Interactive finite element analysis of fracture processes: An integrated
approach. M.S. Thesis, Cornell University, 1987.
 Dolbow J and Gosz M. On the computation of mixed-mode stress intensity factors in
functionally graded materials. International Journal of Solids and Structures, 39(9):2557-
 Kim JH and Paulino GH. T-stress, mixed-mode stress intensity factors, and crack initiation
angles in functionally graded materials: A unified approach using the interaction integral
method. Computer Methods in Applied Mechanics and Engineering, 192(11-12): 1463-1494,
 Paulino GH and Kim JH. A new approach to compute T-stress in functionally graded
materials by means of the interaction integral method. Engineering Fracture Mechanics, 71
 Rice JR. A path-independent integral and the approximate analysis of strain concentration by
notches and cracks. ASME Journal of Applied Mechanics, 35(2):379-386, 1968.
 Yau JF, Wang SS, and Corten HT. A mixed-mode crack analysis of isotropic solids using
conservation laws of elasticity. ASME Journal of Applied Mechanics, 47(2):335-341, 1980.
 Eischen JW. Fracture of non-homogeneous materials. International Journal of Fracture,
 Hussain MA, Pu SL, and Underwood J. Strain energy release rate for a crack under combined
mode I and mode II. In Paris PC and Irwin GR, editors, Fracture Analysis, ASTM STP 560,
pages 2-28, Philadelphia, PA, 1993. American Society for Testing and Materials.
 Rousseau CE and Tippur HV. Compositionally graded materials with cracks normal to the
elastic gradient. Acta Materialia, 48(16):4021-4033, 2000.
 Kim JH and Paulino GH. Simulation of crack propagation in functionally graded materials
under mixed-mode and non-proportional loading,” International Journal of Mechanics and
Materials in Design (in press).